universiti putra malaysia - psasir.upm.edu.mypsasir.upm.edu.my/id/eprint/55702/1/iptph 2014...
Click here to load reader
Post on 28-May-2019
Embed Size (px)
UNIVERSITI PUTRA MALAYSIA
BALKIS FATOMER BINTI A. BAKAR
IPTPH 2014 2
INFLUENCE OF EXTRACTIVES ON THE POROSITY OF OIL PALM (Elais guineensis Jacq.) STEM
INFLUENCE OF EXTRACTIVES ON THE POROSITY OF OIL PALM
(Elais guineensis Jacq.) STEM
BALKIS FATOMER BINTI A. BAKAR
Thesis Submitted to the School of Graduate Studies,
Universiti Putra Malaysia, in Fulfilment of the
Requirements for the Degree of Master of Science
All material contained within the thesis, including without limitation text, logos,
icons, photographs and all other artwork, is copyright material of Universiti Putra
Malaysia unless otherwise stated. Use may be made of any material contained within
the thesis for non-commercial purposes from the copyright holder. Commercial use
of material may only be made with the express, prior, written permission of
Universiti Putra Malaysia
Copyright Universiti Putra Malaysia
To my beloved husband
Nizam Hakim Md. Ishak
My beloved parents
Hj. A. Bakar Othman
Hjh. Farida Amin
My beloved sisters and brother
Thank you for being the people that encouraged me the most.
Abstract of thesis presented to the Senate of Universiti Putra Malaysia in fulfilment of
the requirement for the degree of Master of Science
INFLUENCE OF EXTRACTIVES ON THE POROSITY OF OIL PALM (Elaeis
guineensis Jacq.) STEM
BALKIS FATOMER A. BAKAR
Chairman : Professor Paridah Md. Tahir, PhD
Institute : Institute of Tropical Forestry and Forest Products (INTROP)
In this study, an investigation was conducted to determine the basic properties (moisture
content and density) of the oil palm stem and amount of extractives content that can be
extracted from the sample. Porosity studies were also conducted on the oil palm stem in
different exposure conditions (dried and green) and the influence of extractive on the
porosity was examined. Oil palm trees were selected randomly from the species Elaeis
guineensis Jacq. from Taman Pertanian Universiti located in Universiti Putra Malaysia,
Serdang, Malaysia. Each of the tree were cut along the tree height into three main parts
namely bottom, middle and top. Each part was further cut into three sections labelled as
outer, inner and centre across the transverse direction of oil palm stem. Technical
Association of the Pulp and Paper Industry (TAPPI) standards were employed for water
extractives (cold water and hot water) and also acetone extractives. The green moisture
content of the oil palm stem was found higher at the middle with average of 221.8% and
lowest was at bottom with 158.4%. Across the transverse direction, centre section
always had higher moisture content regardless of the tree height and the lowest was
found at outer section with average of 260.7% and 115.3%, accordingly. The density of
oil palm stem was found inversed with moisture content as the highest density was
found at bottom with average of 0.46 g/cm and the lowest was at middle with 0.37
g/cm. Outer consistently gave higher density compared to centre section with 0.55
g/cm and 0.30 g/cm. The coefficient of determination (R2) obtained between moisture
content and density was high with 0.83. In non-sequential method, hot water extractives
gave higher results compared to other solvents with average of 26.8% of total extracted
compounds. Whereas in the sequential method, cold water was found higher with
average of 21.3%. Comparing the methods, sequential extraction method gave greater
amount of extractives as the samples had gone through three different solvents
continuously. Whilst, parenchyma cells is proven to contribute three times higher of
extractives content compared than vascular bundles.
For theoretical porosity in dried and green condition, samples taken from centre section
at middle part had highest average percentage of 79.4% and 78.2%, respectively and the
least was found at outer section at bottom part with 71.7% and 69.0%, accordingly.
Whereas, experimental porosity was found higher at centre section at top part for dried
condition and at centre section of middle part along the oil palm tree height for green
condition. Experimental porosity surpassed the theoretical porosity values as a result
from the effects of condition exposure of the samples at the upper part of the oil palm
tree (middle and top). However, there is no dependency of extractives content towards
porosity found in this study. This study concluded that moisture content and density of
oil palm stem was affected by the location (longitudinal and transverse direction) of the
sample taken. Extractives content was found higher at sample which consist higher
portion of parenchyma cells. Oil palm stem sample in green condition resulted higher
experimental porosity compared to dried condition. Porosity of oil palm stem has low
influence by its extractives content rather than its anatomical structure. The study
suggests that oil palm stem can be treated by impregnation or preservation process in
Abstrak thesis yang dikemukakan kepada Senat Universiti Putra Malaysia sebagai
memenuhi keperluan untuk ijazah Master Sains
PENGARUH EKSTRAKTIF TERHADAP KELIANGAN BATANG KELAPA
SAWIT (Elaeis guineensis Jacq.)
BALKIS FATOMER A. BAKAR
Pengerusi : Profesor Paridah Md Tahir, PhD
Institut : Institut Perhutanan Tropika dan Produk Hutan (INTROP)
Dalam kajian ini, satu ujikaji telah dijalankan untuk menentukan sifat-sifat asas
(kandungan air dan ketumpatan) daripada batang kelapa sawit dan juga jumlah
kandungan ekstraktif yang boleh diekstrak daripada sampel tersebut. Kajian keliangan
juga dijalankan pada batang kelapa sawit dan pengaruh ekstraktif pada keliangan kayu
dikaji. Pokok kelapa sawit telah dipilih secara rawak daripada spesies Elaeis guineensis
Jacq. dari Taman Pertanian Universiti yang terletak di Universiti Putra Malaysia,
Serdang, Malaysia. Setiap pokok dipotong kepada tiga bahagian utama iaitu bahagian
bawah, tengah dan atas disepanjang ketinggian pokok. Setiap bahagian pula dipotong
menjadi tiga bahagian kecil yang dilabel sebagai luar, dalam dan pusat di arah melintang
batang kelapa sawit. Piawaian (Persatuan Teknikal Industri Pulpa dan Kertas) TAPPI
digunakan untuk eksperimen keterlarutan air (air sejuk dan air panas) dan juga aseton
ekstraktif. Kandungan lembapan hijau batang kelapa sawit didapati lebih tinggi di
tengah dengan purata 221.8% dan terendah adalah di bahagian bawah dengan 158.4%.
Pada arah melintang, bahagian pusat sentiasa mempunyai kandungan lembapan yang
lebih tinggi tanpa mengira ketinggian pokok itu dan yang paling rendah didapati di
bahagian luar dengan purata 260.7% dan 115.3%. Ketumpatan batang kelapa sawit
didapati songsang dengan kandungan lembapan sebagai kepadatan paling tinggi didapati
di bahagian bawah dengan purata 0.46 g/cm dan yang paling rendah adalah di tengah
dengan 0.37 g/cm. Bahagian luar secara konsisten memberikan kepadatan yang lebih
tinggi berbanding dengan bahagian tengah dengan 0.55 g/cm dan 0.30 g/cm. Pekali
penentuan (R2) diperolehi antara kandungan lembapan dan ketumpatan adalah tinggi
dengan 0.83. Dalam kaedah tidak berurutan, keterlarutan air panas memberikan jumlah
yang lebih tinggi berbanding dengan pelarut lain dengan purata sebanyak 26.8%
daripada jumlah sebatian yang diekstrak. Manakala, dalam kaedah berurutan, kelarutan
air sejuk didapati lebih tinggi dengan purata 21.3%. Apabila membandingkan kaedah,
kaedah pengekstrakan berurutan memberikan jumlah yang lebih besar kerana sampel
batang kelapa sawit telah melalui tiga pelarut yang berbeza dalam satu proses.
Tambahan lagi, sel parenkima terbukti menyumbang tiga kali lebih tinggi kandungan
ekstraktif berbanding daripada berkas vaskular.
Untuk teori keliangan dalam keadaan kering dan hijau, sampel yang diambil daripada
bahagian pusat di bahagian tengah mempunyai peratusan tertinggi purata 79.4% dan
78.2% masing-masing dan yang paling didapati di bahagian luar di bahagian bawah
dengan 71.7% dan 69.0%. Manakala, eksperimen keliangan didapati lebih tinggi pada
bahagian tengah di bahagian atas bagi keadaan kering dan di bahagian tengah bahagian
tengah di sepanjang ketinggian pokok kelapa sawit bagi keadaan hijau. Eksperimen
keliangan melepasi nilai teori keliangan sebagai hasil dari kesan pendedahan keadaan
sampel pada bahagian atas pokok kelapa sawit (tengah dan atas). Walau bagaimanapun,
tidak ada pergantungan kandungan ekstraktif terhadap keliangan didapati dalam kajian
ini. Kajian ini mendapati bahawa kandungan lembapan dan ketumpatan batang kelapa
sawit berubah mengikut lokasi sampel (arah ketinggian kelapa sawit dan melintang)
yang diambil. Kandungan ekstraktif didapati lebih tinggi pada sampel yang mempunyai
sel parenkima yang tinggi. Sampel batang kelapa sawit dalam keadaan hijau
menghasilkan bacaan keliangan experiment yang lebih tinggi berbanding keadaan
sampel yang dikeringkan. Keliangan batang kelapa sawit mempunyai pengaruh yang
rendah oleh jumlah ekstraktif berbanding dengan struktur anatomi. Kajian ini juga
mencadangkan bahawa batang kelapa sawit boleh dirawat dalam keadaan hijau.
All praises are due to Allah SWT who had given me blessing, strength and knowledge
in finishing this thesis.
Special notes of gratitude to my main supervisor, Professor Dr Paridah Md Tahir,
without whom my research would not have been possible and completed. I would also
like to thank her for all the guidance and encouragement that she has shown me
throughout the period of this research as a supervisor. To all my committee members
Professor Dr Alinaghi Karimi, and Associate Professor Dr Edi Suhaimi Bakar, I extend
to you my warmest thanks for being patient, understanding and providing me invaluable
guidance. I would like to also say thank you to Professor Dr Zaidon Ashaari, Professor
Dr Salim Hiziroglu and Dr Mohd Khairun Anwar Uyup for your willingness to spend
some time to sharing knowledge with me and guiding me in writing this thesis.
Special thanks to my Head of Department of Forest Production, Dr. Rasmina Halis and
Dean of Faculty of Forestry, Prof. Datin Dr. Faridah Hanum Ibrahim for the approval of
my study leave and all the assistance and advice given. I would also like to extend my
appreciation to all the staff of the Faculty of Forestry and the Institute of Tropical
Forestry and Forest Products, especially Mr Azam, Mr Fakhruddin, Mr Zamani for all
their help during my labwork.
To my fellow researchers, Dr Adrian Choo Cheng Yong, Dr. Juliana Halip, Aisyah
Humaira, Norul Izani, Nor Hafizah, Husna, Lukman, all my ex-UiTM comrades and
other colleagues, I sincerely appreciate all the help that you guys have given to me and I
truly cherish our friendship.
My greatest and deepest gratitude goes to my parents, my parents in law and siblings for
being understanding and supportive through the years. To my husband Hakim, thank
you for always being there for me, being a good listener and encouraging me through
the trials I faced in completing this thesis. I dedicate this thesis to all of you.
I certify that an Examination Committee has met on 27th
May 2014 to conduct the final
examination of BALKIS FATOMER A. BAKAR on her MASTER IN SCIENCE
thesis entitled INFLUENCE OF EXTRACTIVES ON THE POROSITY OF OIL
PALM (Elaeis guineensis Jacq.) STEM in accordance with Universiti Pertanian
Malaysia (Higher Degree) Act 1980 and Universiti Pertanian Malaysia (Higher Degree)
Regulations 1981. The Committee recommends that the student be awarded the relevant
Members of the Examination Committee were as follows:
Azmah Hanim binti Mohamed Ariff, PhD
Faculty of Engineering
Universiti Putra Malaysia
Rasmina binti Halis, PhD
Faculty of Forestry
Universiti Putra Malaysia
Rosfarizan binti Mohamad, PhD
Faculty of Biotechnology and Biomolecular Sciences
Universiti Putra Malaysia
Rokiah Hashim, PhD
School of Industrial Technology
Universiti Sains Malaysia
PROF. DR. ZULKARNAIN
Professor and Deputy Dean
School of Graduate Studies
Universiti Putra Malaysia
This thesis was submitted to the Senate of Universiti Putra Malaysia and has been
accepted as fulfillment of the requirement for the degree of Master of Science. The
members of the Supervisory Committee were as follows
Paridah Md Tahir, PhD
Institute of Tropical Forestry and Forest Products
Universiti Putra Malaysia
Alinaghi Karimi, PhD
Institute of Tropical Forestry and Forest Products
Universiti Putra Malaysia
Edi Suhaimi Bakar, PhD
Faculty of Forestry
Universiti Putra Malaysia
BUJANG BIN KIM HUAT, PhD Professor and Dean
School of Graduate Studies
Universiti Putra Malaysia
Declaration by graduate student
I hereby confirm that:
this thesis is my original work; quotations, illustrations and citations have been duly referenced; this thesis has not been submitted previously or concurrently for any other degree at
any other institutions;
intellectual property from the thesis and copyright of thesis are fully-owned by Universiti Putra Malaysia, as according to the Universiti Putra Malaysia (Research)
written permission must be obtained from supervisor and the office of Deputy Vice-Chancellor (Research and Innovation) before thesis is published (in the form of
written, printed or in electronic form) including books, journals, modules,
proceedings, popular writings, seminar papers, manuscripts, posters, reports, lecture
notes, learning modules or any other materials as stated in the Universiti Putra
Malaysia (Research) Rules 2012;
there is no plagiarism or data falsification/fabrication in the thesis, and scholarly integrity is upheld as according to the Universiti Putra Malaysia (Graduate Studies)
Rules 2003 (Revision 2012-2013) and the Universiti Putra Malaysia (Research)
Rules 2012. The thesis has undergone plagiarism detection software.
Signature: _______________________ Date: __________________
Name and Matric No.: _________________________________________
Declaration by Members of Supervisory Committee
This is to confirm that:
the research conducted and the writing of this thesis was under our supervision; supervision responsibilities as stated in the Universiti Putra Malaysia (Graduate
Studies) Rules 2003 (Revision 2012-2013) are adhered to.
Name of Name of
Chairman of Member of
TABLE OF CONTENTS
LIST OF TABLES xiii
LIST OF FIGURES xiv
LIST OF ABBREVIATIONS xvii
1 INTRODUCTION 1
1.1 General view 1
1.2 Problem Statement 2
1.3 Objectives 3
2 LITERATURE REVIEW 4
2.1 Introduction 4
2.2 General Description of Oil Palm 4
2.3 Oil Palm Biomass 7
2.4 Morphology Characteristics of Oil Palm Stem 8
2.5 Anatomical Features of Oil Palm Stem 8
2.5.1 Vascular Bundles 10
2.5.2 Parenchyma 10
2.6 Physical Properties of Oil Palm Stem 11
2.6.1 Density 12
2.6.2 Moisture Content 13
2.7 Chemical Composition of Oil Palm Stem 14
2.7.1 Extractives 15
2.7.2 Extractives Content in Oil Palm Stem 15
2.7.3 Classification of Wood Extractives 16
2.7.4 Techniques of Extraction 17
2.8 Porosity 18
2.8.1 Fluid Flow in Lignocellulosic Materials 18
2.8.2 Moisture in Oil Palm Stem 21
2.8.3 Determination of Porosity 23
2.8.4 Effect extractives content towards porosity 23
3 METHODOLODY 25
3.1 Material Selection 25
3.2 Experimental Design 26
3.3 Determination of Moisture Content 28
3.4 Determination of Density 28
3.5 Determination of Extractives Content 28
3.5.1 Acetone Extractives 30
3.5.2 Cold Water Extractives 30
3.5.3 Hot Water Extractives 31
3.5.4 Non-Sequential and Sequential Extraction 31
3.5.5 Non- sequential extraction of Vascular 31
Bundles and Parenchyma
3.6 Porosity of Oil Palm Stem 32
3.7 Statistical Analysis 34
4 RESULTS AND DISCUSSION 35
4.1 Moisture Content and Density of Oil Palm Stem 35
4.1.1 Moisture Content 35
4.1.2 Density 37
4.2 Extractives Content in Oil Palm Stem for 39
Non-Sequential Extraction Process
a) Acetone Extractives 40
b) Water Extractives (Cold and Hot Water Solubility) 41
4.3 Extractives Content in Oil Palm Stems for 44
Sequential Extraction Process
a) Cold Water Extractives 45
b) Hot Water Extractives 46
c) Acetone Extractives 48
4.4 Determination of Extractives Content in Vascular Bundles 51
4.5 Investigation on Oil Palm Stem Porosity 52
5 CONCLUSION AND RECOMMENDATIONS 67
5.1 Conclusion 67
5.2 Recommendations 68
BIODATA OF STUDENT 88
LIST OF PUBLICATIONS 89
LIST OF TABLES
2.1 Oil palm taxonomy 4
2.2 Properties of a 27 year old oil palm stem at various sections 11
and height of the stem.
2.3 Chemical composition in different wood species 14
2.4 Techniques of extractions and corresponding extracted compounds 17
3.1 Summaries of replicates used for the experimental work 26
4.1 Analysis of variance of the effect between height and section 35
on the density and moisture content of oil palm stem
4.2 Comparison of moisture content of oil palm tree at different 36
ages (14, 25 and 32 years)
4.3 Analysis of variance for the effects of tree height and sections 39
on the yields of different types of extractives
4.4 Analysis of variance of extractives yields for different height 45
and sections within the stem using 3 different solvent using
sequential extraction method
4.5 Analysis of variance (ANOVA) for theoretical porosity and 52
experimental porosity of oil palm stem
LIST OF FIGURES
2.1 Transverse section of oil palm stem 5
2.2 Sample taken along the transverse direction of oil palm stem indicated 6
as a) outer section b) inner section and c) centre section.
2.3 Estimated percentage of oil palm biomass 7
2.4 Sample was taken from bottom part. Darker section is represent 9
as outer which having compact vascular bundles and lighter
colour at centre section where the parenchyma is dominant
2.5 Vascular bundles and parenchyma of oil palm stem (5x magnification) 9
2.6 Schematic diagram of density variation in oil palm stem 12
2.7 Extractives classification 16
2.8 Samples were cut into two to observed the penetration of acid fuchsin 19
after 16 h of immersion
2.9 SEM images showing the differences anatomical structure of 20
a) hardwood, b) softwood, c) oil palm stem
2.10 The three principal axes of wood 22
3.1 Schematic labelling of oil palm stem 25
3.2 General view of experimental design in this study 27
3.3 Sample preparation from oil palm billet to form a board 29
3.4 The oil palm billet was cut into stick form (2 x 2 x length in diameter) 29
3.5 Oil palm stem particles weighted 2 g each for extraction process 30
3.6 Vascular bundles and parenchyma cells were separated for further 32
3.7 Schematic diagram to prepare blocks in two different condition 32
3.8 Sample size (2 x 2 x 2 cm) of oil palm stem 32
3.9 Summary of process flow for porosity test 33
4.1 Moisture content in longitudinal and transverse sections of oil palm stem 36
4.2 Density in longitudinal and transverse sections of oil palm stems 38
4.3 Correlation between density and moisture content of oil palm stem 39
4.4 Extractives in longitudinal and transverse directions of oil palm stem 40
dissolved in acetone
4.5 Extractives in longitudinal and transverse directions of oil palm stem 41
dissolved in cold water
4.6 Extractives in longitudinal and transverse directions of oil palm stem 42
dissolved in hot water
4.7 Mapping of the distribution of extractives content in the oil palm stem 44
using a) acetone, b) cold water and c) hot water
4.8 Extractives in longitudinal and transverse directions of oil palm stem 45
dissolved in cold water for sequential extraction
4.9 Distribution of vascular bundles and parenchyma cells in a) outer and 46
b) centre section of bottom part of oil palm stem
4.10 Extractives in longitudinal and transverse directions of oil palm stem 47
dissolved in hot water for sequential extraction
4.11 Starch found in parenchyma cells at a) bottom outer and b) top centre 48
section of oil palm stem
4.12 Extractives in longitudinal and transverse directions of oil palm stem 49
dissolved in acetone for sequential extraction
4.13 Extractives content in average percentage between non-sequential and 50
sequential extraction process
4.14 Extractives in vascular bundles and parenchyma cells using three 51
4.15 Theoretical porosity in oil palm stem (longitudinal and transverse) as 53
function of conditions
4.16 Crack occurred and hollow space observed at parenchyma cells of oil 54
palm stem using Dino Light with 65x magnification
4.17 Experimental porosity in oil palm stem (longitudinal and transverse) 55
as function of condition
4.18 Comparison between theoretical and experimental porosity for bottom 57
height along the transverse direction of oil palm stem in dried condition
4.19 Difference occurrence of vascular bundles at outer section taken from 57
bottom (left) and middle (right) with sample size 2x2x2 cm each
4.20 Comparison between theoretical and experimental porosity for bottom 58
height along the transverse direction of oil palm stem in green condition
4.21 Comparison between theoretical and experimental porosity for middle 59
height along the transverse direction of oil palm stem in dried condition
4.22 Comparison between theoretical and experimental porosity for middle 60
height along the transverse direction of oil palm stem in green condition
4.23 Comparison between porosity and free water for top height along the 61
transverse direction of oil palm stem in dried condition.
4.24 Effect of drying process on oil palm samples across the transverse 62
direction of the stem
4.25 Outer section at top height sample shows some of the defects resulted 62
4.26 Comparison between theoretical and experimental porosity for top height 63
along the transverse direction of oil palm stem in green condition
4.27 Starch granule in the top part of oil palm stem 64
4.28 Correlation between theoretical porosity and extractives content of oil 65
palm stem in dried condition
4.29 Correlation between theoretical porosity and extractives content of oil 65
palm stem in green condition
4.30 Correlation between experimental porosity and extractives content of 66
oil palm stem in dried condition
4.31 Correlation between experimental porosity and extractives content of 66
oil palm stem in green condition
LIST OF ABBREVIATIONS
(-OH) hydroxyl groups
ANOVA Analysis of variance
CPO Crude palm oil
EFB Empty fruit bunch
EMC Equilibrium moisture content
FSP Fibre saturation point
GBP Gympsum-bonded particleboard
Lmw PF Low molecular weight phenol formaldehyde
LSD Least significant difference
LVL Laminated veneer lumber
MDF Medium-density fibreboard
MF Mesocarp fibre
MIDA Malaysian Industrial Development Authority
MPOB Malaysian Palm Oil Board
PKO Palm kernel oil
PKS Palm kernel shells
POME Palm oil mill effluent
R Coefficient of determination
SAS Statistical analysis variance
TAPPI Technical Association of the Pulp and Paper Industry
TPU Taman Pertanian Universiti
1.1 General View
Since early 1960s, the cultivation of oil palm plantation increased at a fast pace in
line with the governments agricultural diversification program, which was
introduced to reduce the countrys economic dependence on rubber and tin (Rasiah
and Shahrin, 2004). Later in the 1960s, the government introduced land settlement
schemes for planting oil palm tree to eliminate poverty for the landless farmers and
smallholders. Initially, oil palm tree was planted to harvest the palm oil from its
fruits. The latest statistical data extracted from MPOB (2014) had reported that there
was 5.23 million ha of oil palm plantation in 2013 compared to 5.08 million ha in
2012. The largest oil palm plantation was dominated by Peninsular Malaysia with
2.59 million ha, followed by Sabah (1.48 million ha) and Sarawak (1.16 million ha)
In spite of substantial plantation, ample oil palm stems are available during
replanting process which happens after the trees reach 25 to 30 years. The stems
generated approximately 15.39 million tonnes of lignocellulosic materials annually
(Hartono, 2012).Previously, the discarded stems were burnt in the field as disposal of
the wastes (Lim and Gan, 2005) or were left at the oil palm plantation as natural
With proper treatment against bio-deteriorating agents, the oil palm stems have been
proven to be used in various applications such as laminated veneer lumber (LVL)
and plywood (Loh et al., 2011; Sulaiman et al., 2008: Nordin et al., 2004) are used as
the core materials to produce framing materials for the manufacture of furniture. Oil
palm stem usage is extended as well as to other composite panels, such as
particleboard, medium-density fibreboard (MDF) and wood cement board. Rahim
and Khozirah (1991) had introduced gympsum-bonded particleboard (GBP) by using
fresh oil palm stem chips. Additionally, recent works done by several authors
(Hoong et al., 2013; Nor Hafizah et al., 2012; Loh et al., 2011) had produced high
grade oil palm plywood and veneers by impregnated low molecular weight phenol
formaldehyde (LmwPF) into the samples.
However, there is no economic value of oil palm stem from structural point of view
(Abdul Khalil, 2006), and the maximum utilization of oil palm stem still constrained
with several factors such as variation in density (Loh et al., 2011; Choo et al., 2010;
Bakar et al., 2008; Lim et al., 2003), high moisture content (Bakar et al., 2008;
Shirley, 2002), high extractives content (Darmawan, 2006) and low dimensional
stability (Bakar et al., 2008; Ibrahim, 1989). Therefore, various techniques have been
implemented to enhance the properties of oil palm stem end products through
polymer injection (Zugenmaier, 2006; Ibrahim, 1989), thermal treatment (Fukuta,
2008; Higashihara et al., 2000), chemical modification (Mahlberg et al.,2001; Xie et
al., 2007) and resin impregnation (Nor Hafizah et al., 2014; Bakar et al., 2013 and
2008; Hoong et al., 2012; Loh et al., 2011; Irshad et al., 2010).In general, such
processes aim to improve the weather and decay resistance, dimensional stability,
strength, colour and paintability properties of materials (Herajarvi, 2009).
Most of the treatments particularly using chemical treatments are related to the basic
properties of the woody or lignocellulose such as porosity and permeability value.
Like wood, oil palm stem is a porous material (Kollmann and Cote, 1968) which
composed of cell wall substances and cavities containing air and extractives
(Tsoumis, 1991). The specific gravity of the cell wall practically constant for all
woody material with value of 1.53 g/cm3 on an oven dry mass and volume basis, and
the cell wall materials are completely non-porous (Dinwoodie, 1981). What make oil
palm stem differ from other wood such as rubberwood is it belongs to
monocotyledon plants which means oil palm stem does not possess any vascular
cambium, secondary growth, growth rings, ray cells, sapwood and heartwood,
branches and knots (Killmann and Lim, 1985) compared to dicotyledon plants. Flow
of fluid in oil palm stem is mainly through metaxylem vessels in vascular bundles
(Shirley, 2002) and several researchers also found that parenchyma contributes to
absorb more liquid as it have thin walled and high absorbency rate (Nordin, 2012;
Paridah et al., 2006).
Moreover, oil palm stem is a much more porous, cellular and anisotropic in nature.
Thus liquid such as water and low molecular weight compounds can rapidly
absorbed and flow into the cell wall and lumen (Loh et al., 2011). Basically, wood
porosity can ranged from 46 to 80% of total wood volume which can give significant
effect to the depth and direction of fluid flows like preservatives and adhesives in
treatment process (Vick, 1999). During the treatment process, penetration of liquid in
wood pores depends on surface roughness, density, extractives content and properties
of the liquid itself (Nor Hafizah et al., 2012). Oil palm stem also has been reported to
contain high extractives content (10%) compared to other wood (Darmawan, 2006),
and Olsson et al. (2001) believed that extractives are one of the main reasons for
reduced transverse permeability of pine heartwood.
1.2 Problem Statement
Lignocellulosic material is chemically heterogeneous and its components can be
divided into two groups; structural components of high molecular weight which
includes cellulose, hemicellulose and lignin that contributes to the major cell wall
components; and non-structural components of low molecular weight (extractives
and inorganic components). The extractives are non-polymeric and may be separated
from the insoluble cell wall materials by solving them in water or organic solvents
(Vaicklenionis and Vaickelioniene, 2006). In general, the overall percent of the
extractives in wood varies from 2 to 10% and oil palm stem consists the highest
extractives content among other monocotyledon plants (Darmawan, 2006). The
effects of extractives resulted in corrosion of metals in contact with wood, inhibition
of setting of concrete, glue and finishes (David and Nobuo, 2001). During the drying
process, extractives that presence in wood are transported to the surface in a
heterogeneous distribution and deposited as solids when the water evaporates
causing the interference with absorption and curing process of the substances.
Contamination of wood surface by having heavy deposits of extractives may reduce
bonding strength by blocking the reaction sites and prevent true wetting by the
adhesives (Hse and Kuo, 1988).
Moreover, Behr et al. (2011) stated that in Scots pine, extractives are believed to be
one of the main reason for the reduced transverse permeability of pine heartwood. A
small amount of distributed extractives is enough to encrust the bordered pits
permanently and block them for liquids as extractives were related to reduce wood
treatability (Zimmer et al., 2009). A vast number of experimental results have shown
that the removal of extractives increases the dimensional changes of wood
(Adamopoulos and Voulgaridis, 2012; Stamm and Loughborough, 1942). In study
done by Adamopoulos and Voulgaridis (2012) on Black Locust wood had found that
removal of extractives also resulted to a slight gradual increase in radial and
tangential dimensional changes of the wood. Furthermore, Darmawan et al. (2012)
reported that wood extractives and silica have a potential adverse effect on tool wear.
As in wood, the most crucial properties determining the ease of drying and treatment
in oil palm stem is its porosity. Porosity is the fractional of void volume of wood and
to be a permeable, a solid must be porous (Siau, 1984). However, having high
porosity values does not mean that the material will have higher permeability values
as a result from blockage or cell ruptured. The knowledge of porosity is important as
a factor influencing the amount of liquid that can be absorbed in a given block
volume and influenced the way preservative retention is expressed (Usta, 2006). For
instance, the maximum amount of treating solution that can be injected into wood
can be determined. Research on porosity has always been highlighted on the
hardwoods and softwoods as compared to monocotyledons (Nordin, 2012; Plotze and
Niemz, 2011). Only limit information has been found for porosity of oil palm stem
and it is not sufficient to help boost the effect of the treatment that using liquid. Thus,
hypothesis for this study is wood extractives that are presence in oil palm stem may
block the voids in liquid absorption of oil palm stem.
The main objective of this study was to evaluate the influence of extractives on the
porosity of oil palm stem.
Specific objectives of the work were:
a) To determine the moisture content and density of oil palm stem along the tree height and transverse section.
b) To evaluate the extractives content in longitudinal and transverse section of oil palm stem.
c) To determine the porosity relationships with extractives content of oil palm stem along the tree height and transverse direction.
Abdul Khalil, H.P.S., Hanida, S. Kang, C.W., and Nik Fuaad, N.A. (2007). Agrohybrid
Composite: The Effects on Mechanical and Physical Properties of Oil Palm Fiber
(EFB)/ Glass Hybrid Reinforced Polyester Composites. Journal of Reinforced
Plastics and Composites 26(2): 203-218.
Abdul Khalil, H.P.S., Nurul Fazita, M.R., Bhat, A.H., Jawaid, M., and Nik Fuad, N.A.
(2010). Development and Material Properties of New Hybrid Plywood from Oil
Palm Biomass. Materials and Design 31(1): 417-424.
Abdul Khalil, H.P.S., Siti Alwani, M., Mohd Omar A.K. (2006). Chemical Composition,
Anatomy, Lignin Distribution, and Cell Wall Structure of Malaysian Plant Waste
Fibers. Bioresources 1(2): 220-232.
Abdullah, C.K., Jawaid, M., Abdul Khalil, H.P.S., Zaidon, A., and Hadiyane, A. (2012). Oil
Palm Trunk Polymer Composite: Morphology, Water Absorption, and Thickness
Swelling Behaviours. Bioresources 7(3): 2948-2959.
Abdullah, N., Sulaiman, F., and Gerhauser, H. (2011). Characterisation of Oil Palm Empty
Fruit Bunches for Fuel Application. Journal of Physical Sciences 22(1): 1-24.
Abe, H., Murata, Y., Kubo, S., Watanabe, K., Tanaka, R., Sulaiman, O., Hashim, R., Sitti
Fatimah, M.R., Zhang, C., Noshiro, S., and Mori, Y. (2013). Estimation of the Ratio
of Vascular Bundles to Parenchyma Tissue in Oil Palm Trunks Using NIR
Spectroscopy. Bioresources 8(2): 1573-1581.
Adamopoulos, S and Voulgaridis, E. (2012). Effect of Hot-Water Extractives on Water
Sorption and Dimensional Changes of Black Locust Wood. Wood Research 57(1):
Ahmad, Z, Saman, H.M., and Paridah, M.T. (2010). Oil Palm Trunk Fiber as a Bio-Waste
Resource for Concrete Reinforcement. International Journal of Mechanical and
Materials Engineering (LIMME) 5(2): 199-207.
Ali, R. A. S. and Halim, A. H. (1991). The Fffect of Oil Palm Wood Extractives on Growth
of Decaying Microorganisms. Proceedings Oil Palm Trunk and Other Palmwood
Utilization, Malaysia, Kuala Lumpur p73-80.
Antwi-Boasisko, C. & Pitman, A.J. (2009) .Influence of Density on The Durabilities of
Three Ghanaian Timbers. Journal of Science and Technology, Vol. 29, No. 2. DOI
Anwar, U.M.K., Zaidon, A., Hamdan, H., and Mohd Tamizi, M. (2005). Physical and
Mechanical Properties of Gigantochloa scortechinii Bamboo Splits and Strips.
Journal of Tropical Forest Science 17(1): 413-418.
Ari, L.H. (2005). Solubility of Structurally Complicated Materials: 1. Wood. Journal
Physics and Chemistry References Data 35(1): 77-91.
Back, E. L. (1960) On the Relative Composition of Canal Resin and Ray Parenchyma Resin
in Picea Abies (Karst.) Stemwood. The Resin in Parenchymatous Cells and Resin
Canals of Conifers. Svensk Papperstidning 63 (19):647-651.
Back, E.L. (1991). Oxidation Activation of Wood Surfaces for Glue Bonding. Forest
Product Journal 41(2): 30-36.
Bakar, E.S. (2000). Utilization of Oil Palm Trunk as Housing and Furniture Material.
Project Report. Unpublished.
Bakar, E.S., Mohd Hamami, S. and Hng, P.S. (2008). Anatomical Characteristics and
Utilization of Oil Palm Wood. In: Nobuchi, T., Mohd. Hamami, D (Eds) the
Formation of Wood in Tropical Forest Trees: A Challenge from the Perspective of
Functional Wood Anatomy. Malaysia, Universiti Putra Malaysia, Serdang: Academic
Bakar, E.S., Paridah, M.T., and Shahri, M.H. (2005). Properties Enchancement of Oil Palm
Wood through the Compreg Method. Proceeding International Symposium of Wood
Science and Technology 2: 91-92
Bakar, E.S., Paridah, M.T., Fauzi, F., Mohd, H.S. and Tang, W.C. (2007). Properties
Enhancement of Oil Palm Wood through Modified Compreg Method: A
Comprehensive Solution to Oil Palm Woods Properties Flaws (pp 99-112).
Utilization of Oil Palm Tree: Strategizing for Commercial Exploitation.
Bakar, E.S., Rachman, O., Darmawan, W., and Hidayat, I. (1999). Utilization of Oil Palm
Trees as Building and Furniture Material (II): Mechanical Properties of Oil-palm
Wood. Journal Teknologi Hasil Hutan, Fakulti Hutan IPB. Vol.XII (1): 10-20.
Bakar, E.S., Tahir, P.M., Sahri, M.H., Mohd Noor, M.S., Zulkifli, F.F. (2013).
Properties of Resin Impregnated Oil Palm Wood (Elaeis Guineensis Jacq). Pertanika
Journal Tropical Agricultural Science 36(S): 93-100.
Behr, G., Larnoy, E. and Bues, C.T. (2011). Treatability variation of Scots pine Heartwood
from Northern Europe. 42nd
Annual Meeting, Queenstown, New Zealand.
BFPIC. (2009). Beijing Forestry and Parks Department of International Cooperation.
Boustingorry, P. Grosseau, P. Guyonnet, R. and Guilhot, B. (2005). The Influence of Wood
Aqueous Extractives on the Hydration Kinetics of Plaster. Cement and Concrete
Research 35(11): 2081-2086.
Brazier, J.D. and Howell, R.S. (1979). The Use of a Breast Height Core for Estimating
Selected Whole Tree Properties of Stika Spruce. Forestry 52(2): 177-185.
Brown, H.P., Panshin, A.J. and Forsaith, C.C. (1952). Textbook of Wood Technology. Vols 1
& 2. Mcgraw-Hill Book Company Inc. London.
Butterfield, B.G., and Meylan, B.A. (1980). Three-dimensional Structure of wood- An
Ultrastructure Approach. The 2nd
Pacific Regional Wood Anatomy Conference Forest
Products Research and Development Institute Los Banos (College), Lahuna,
Cave, I.D., and Walker, J.C.F. (1994). Stiffness of Wood in Fast-Grown Plantation
Softwoods: The Influence of Microfibril Angle. Forest Products Journal 44(5): 43-
Chen, C.M. (1970). Effects of Extractive Removal on Adhesion and Wettability of Some
Tropical Woods. Forest Product Journal 20(1):36-41.
Choo, A.C.Y. (2012). Permeability and Moisture Distribution in Oil Palm Wood and Its
Influence on the Development of an Effective Method for Veneer Moisture Reduction.
PhD. Thesis. Universiti Putra Malaysia, Malaysia.
Choo, A.C.Y., Paridah, M.T., Karimi, A., Bakar, E.D., Khalina, A., Azmi, I., Loh, Y.F.
(2010) Density and Humidity Gradients in Veneers of Oil Palm Stems. European
Journal Wood Product. DOI 10.1007/S00107-010-0483-1.
Choo, A.C.Y., Paridah, M.T., Karimi, A., Bakar, E.S., Khalina, A., Azmi, I., Balkis
Fatomer, A.B. (2013). Study on the Longitudinal Permeability of Oil Palm Wood.
Industrial and Engineering Chemistry Research 52(27): 9405-9410.
Christianse, A.W. (1994). Effect of Ovendrying of Yellow-Poplar Veneer on Physical
Properties and Bonding. Holz Roh- Werkstoff 52: 139-149.
Cown, D.J., Young, G.D., and Burdon, R.D. (1992). Variation in Wood Characteristics of
20-year-old-half-sib Families of Pinus Radiata. N.Z Journal of Forestry Science 22:
Darmawan, W., Rahayu, I. S., Nandika, D., and Marchal, R. (2012). The Importance of
Extractives and Abrasives in Wood Materials on the Wearing of Cutting Tools.
Bioresources 7(4): 4715-4729.
Darmawan, W., Rahayu, I.S., Tanaka, C. and Marchal, R. (2006). Chemical and Mechanical
Wearing of High Speed Steel and Tungsten Carbide Tools by Tropical Woods.
Journal of Tropical Forest Science, 18(4), 255-260.
David, H.N.S., and Nobuo, S. (2001). Wood and Cellulosic Chemistry, 2nd
ed. p.914, Marcel
Dekker, Inc., New York.
Dinwoodie, J.M. (1981). Timber: Its structure, Properties and Utilisation. 410. London. 6th
edition. MacMillan Press Ltd.
Erwinsyah. (2008). Improvement of Oil Palm Trunk Properties using Bioresin. PhD.
Dissertation. Faculty of Environment Sciences, Technische Universitas Dresden,
Fengel, D. and Wegener, G. (1984). Wood: Chemistry, Ultrastructure Reactions, New York:
Walter de Gruyter.
Fernandez, M.P., Watson, P.A., Breuil, C. (2001). Gas Chromatography-Mass Spectrometry
Method for the Simultaneous Determination of Wood Extractive Compounds in
Quaking Aspen. Journal of Chromatography a 992:225-233.
Findlay. W.P.K. 1975. Preservative of Timber in the Tropic. Martinus Nijhoff/Dr
Foo, Y.N., Foong, K.Y., Basiron, Y, Sundram, K. (2011). A Renewable Future Driven with
Malaysian Palm Oil-based Green Technology. Journal of Oil Palm and the
Fukuta, S., Asada, F., and Sasaki, Y. (2008). Manufacture of Compressed Wood Fixed by
Phenolic Resin Impregnation through Drilled Holes. Journal Wood Science 54(2):
Gardner, D.J., Wolcott, M.P., Wilson, L., Huang, Y., and Carpenter, M. (1995). Our
Understanding of Wood Surface Chemistry. Proceeding No. 7296. Wood Ahdesives.
Forest Products Society, Madison, WI, USA. p29-36
Grabner, M., Muller, U, Gierlinger, N and Wimme, R. (2005). Effects of Heartwood
Extractives on Mechanical Properties of Larch. IAWA Journal 26(2): 211-220.
Grioui, N., Haloui, K., Zoulalian, A., Halouani, F. (2007). Experimental Study on Thermal
Effect on Olive Wood Porous Structure During Carbonization. Maderas. Ciencia y
Tecnologia 9(1): 15-28.
Golpayegani, A.S., Thevenon, M.F., Gril., J., Masson, E., and Pourtahmasi, K. (2014).
Toxicity Potential in the Extraneous Compounds of White Mulberry Wood (Morus
alba). Maderas, Science of Technology 16(2): 227-238.
Hancock, W. V. (1963). Effect of Heat Treatment on the Surface of Douglas-Fir Veneer.
Forest Product Journal 13(2): 81-88.
Harold, P. (1998). Conservation of Architectural Heritage, Historic Structures and
Hartley, C.W.S. (1977). The Oil Palm. Third Edition, Longmans, Green and Co. Ltd.
London. 37 49.
Hartono, R. (2012), Quality Enhancement of Oil Palm Trunk of Inner Part by Close System
Compression Method and Compregnation Phenol Formaldehyde. Bogor Agricultural
University. School of Postgraduate. Bogor Agricultural University.
Hashim, R, Nadhari, W.N.A.W., Sulaiman, O., Kawamura, F., Hiziroglu, S., Sato, M.,
Sugimato, T., Tay, G.S., and Tanaka, R. (2011). Characterization of Raw Materials
and Manufactured Binderless Particleboard from Oil Palm Biomass. Material and
Haslett, A.N. (1990). Suitability of Oil Palm Trunk for Timber Uses. Journal of Tropical
Forest Science, 2 (5). 245-251.
Henson, I. E., Chang, K. C., Siti Nor Aisyah, M., Chai, S.H.,Hasnuddin Mhd, Y. and
Zakaria, A. (1999) The Oil PalmTrunk as a Carbohydrate Reserve.
Herajarvi, H. (2009). Effect of Drying Technology on Aspen Wood Properties. Silva
Fennica 43(3): 433-445.
Higashihara, T., Morooka, T., and Norimoto, M. (2000). Permanent Fixation of Transversely
Compressed Wood by Steaming and Its Mechanism. Mokuzal Gakkaishi 46(4): 291-
Hillis, W.E. (1971). Distribution, Properties and Formation of Somewood Extractives. Wood
Sciences and Technology, Vol. 5, 272-289.
Hishamudin, M.J. (1987). The Oil Palm Industry in Malaysia. A Guide Book. Palm Oil
Research Institute of Malaysia. Bangi.
Holmbom, B. (1993). Chapter 5 Extractives. Book of Analytical Methods in Wood
Chemistry, Pulping, and Papermaking (pp 125) by Eero Sjstrm, Raimo Aln.
Hong, L.T. and Killman, W. (1989). Some Aspects of Parenchymatous Tissues in Palm
Stems. The 2nd
Pacific Regional Wood Anatomy Conference, Forest Products
Research and Development Institute Los Banos (College), Laguna, Philippines. 449-
Hoong, Y.B., Loh, Y.F., Chuah, L.A., Juliwar, I., Pizzi, A., Paridah, M.T., and Jalaluddin,
H. (2013). Development a New Method for Pilot Scale Production of High Grade Oil
Palm Plywood: Effect of Resin Content on the Mechanical Properties, Bonding
Quality and Formaldehyde Emission of Palm Plywood. Materials and Design 52:
Hoong, Y.B., Loh, Y.F., Nor Hafizah, A.B., Paridah, M.T., and Jalaluddin, H. (2012).
Development of a New Pilot Scale Production of High Grade Oil Palm Plywood:
Effect of Pressing Pressure. Materials and Design 36: 215-219.
Hse, C.Y. and Kuo, M.L. (1988). Influence of Extractives on Wood Gluing and Finishing-A
Review http://www.iccrom.org/pdf/ICCROM_14_ARCLab Handbook01_en.pdf.
Ibrahim, M. M., Agblevor, F. A., and El-Zawawy, W. K. (2010). Isolation and
Characterization of Cellulose and Lignin from Steam-Explode Lignocellulosic.
Biomass. Bioresources 5: 397-418
Ibrahim, W.A. (1989). Densification and Stabilization of Oil Palm Stem by Treatment with
Two Polymers. Journal of Tropical Forest Science 2(1):1-7.
Irshad, H.B., Abdullah, C.K., Abdul Khalil, H.P.S., Hakimi Ibrahim, M., and Nurul Fazita,
M.R. (2010). Properties Enhancement of Resin Impregnated Agro Waste: Oil Palm
Trunk Lumber. Journal of Reinforced Plastics and Composites 29(22): 3301-3308.
ITIS. (2007). Integrated Taxonomic Information System. Standard Report Page: Elaeis
guineensis. http://www.itis.gov/servlet/SingleRpt/SingleRpt, May 2007.
Izekor, D.N., Fuwape, J.A., and Oluyege, A.O. (2010). Effects of Density on Variations in
the Mechanical Properties of Plantation Grown Tectona Grandis Wood. Applied
Science Research 2(6): 113-120.
Jaqoc, R.B. (1952). Oil Palm and Early Introduction of Elaies guineensis to Malaya.
Malaysia Agriculture Journal 35: 3-10.
Jordon, D.L., and Wellons, J.D. (1977). Wettability of Dipterocarp veneers. Wood Science
Kasemsiri, P., Hiziroglu, S., Rimdusit, S. (2012). Characterization of Heat Treated Eastern
Redcedar (Juniperus virginiana L.). Journal of Material Process Technology 212:
Khalil, A.S., Alwani, M.S., Omar, A.M. (2006). Cell Wall of Tropical Fibers. Bioresources
Kilic, A. and Niemz, P. (2010). Extractives in Some Tropical Woods. European Journal
Wood Product, DOI 10.1007/S00107-010-0489-8.
Killmann, W. and Lim, S.C. 1985. Anatomy and Properties of Oil Palm Stem. Proceedings
of the National Symposium of Oil Palm By-Products for Agro based Industries,
Kuala Lumpur. PORIM Bulletin no. 11: 18-42.
Kocaefe, D., Shi, J.L, Yang, D.Q., Bouazara, M. (2008). Mechanical Properties,
Dimensional Stability, and Mold Resistance of Heat-Treated Jack Pine and Aspen.
Forest Product Journal 58: 88-93.
Kollmann, F.F.P., and Cote, W.A. (1968). Principles of Wood Science an Technology (I).
Solid Wood. p592. Berlin. Springer-Verlag.
Leofanti, G., Padovan, M., Tozzola, G., and Venturelli, B. (1998). Surface Area and Pore
Texture of Catalysts. Catalysis Today 41(1-3): 207-219.
Li, X. (2004). Physical, Chemical and Mechanical Properties of Bamboo and Its Utilization
Potential for Fiberboard Manufacturing. Master Thesis. Louisiana State University,
Liang, C., Zhan, H., Li, B., and Fu, S. (2011). Characterization of Bamboo SCMP Alkaline
Extractives and the Effects on Peroxide Bleaching. Bioresources 6(2): 1484-1498.
Liese, W. (1980). Anatomy of Bamboo in Lessard, G. Sc Chouinard, A. (Eds.) Bamboo
Research in Asia. Proceedings of the Seminar on Bamboo in Asia. pp. 161-164.
Lim, S.C. and Gan, K.S. (2005). Characteristics and Utilization of Oil Palm Stem. Timber
Technology Bulletin 25. ISSN p139-258.
Lim, S.C., and Khoo, K.C. (1986). Characteristics of Oil Palm Trunk and Its Potential
Utilisation. The Malaysian Forester 49(1):3-21.
Lim, S.C., Gan, K.S., and Choo, K.T. (2003). The Characteristics Properties and Uses of
Plantation Timbers-Rubberwood and Acacia Mangium. Timber Technology Bulletin
26. ISSN p139-258.
Loh, Y.F., Paridah, M.T., Hoong, Y.B., Choo, A.C.Y. (2011). Effects of Treatment with
Low Molecular Phenol Formaldehyde Resin on the Surface Characteristics of Oil
Palm (Elaeis quineensis) Stem Veneer. Materials and Design 32: 2277-2283.
Lu, J.Z., Wu, Q., and Negulescu, I.I. (2002). The Influence on Maleation on Polymer
Adsorption and Fixation, Wood Surface Wettability, and Interfacial Bonding
Strength in Wood- PVC Composites. Wood Fibre Science 34(3). 434-459.
Mahlberg, R., Paajanen, L., Nurmi, A., Kivisto, A., Koskela, K. and Rowell, R.M. (2001).
Effect of Chemical Modification of Wood on the Mechanical and Adhesion
Properties of Wood Fiber/Polypropylene Fiber and Polypropylene/Veneer
Composites. Holz als Roh un Werkstoff 59: 319-326.
Malik, J. and Santoso, A. (2011). Effect of Extractive-Dissolving Treatment on the
Characteristics of Laminated Wood Assembled from Oily Keruing Wood. Journal of
Agricultural Science and Technology B 1: 1191-1196.
Mantanis, G.I., Young, R.A., and Rowell, R.M (1995). Swelling of Wood. Part III. Effect of
Temperature and Extractives on Rate and Maximum Swelling. Holzforschung
Margot, S.P. (2005). Properties of Solid Wood. Responses to Drying and Heat Treatment.
Licentiate Thesis. Lulea University of Technology, Sweden.
Mohd Husin, Zin, Z.Z., and Halim, A.H. (1985). Potentials of oil palm by-products as Raw
Materials for Agro-Based Industries. Proceedings of the National Symposium on Oil
Palm By-Products for Agro-Based Industries. Palm Oil Research Institute of
Mohd Zin, J. and Imamura, Y. (1989). Anatomical Characterization of Vascular Bundles in
Oil Palm Trunks. The 2nd Pacific Regional Wood Anatomy Conference Forest
Products Research and Development Institute Los Banos (College), Lahuna,
Mohd. Nor, M.Y., Khoo, K.C., and Lee, T.W. (1984) Preliminary Characterization of Oil
Palm Stem as Raw Material for Pulp and Paper. The Malaysian Forester
MPOB. (2014). Malaysia Palm Oil Board (MPOB). Economics and Statistics. Accessed
1st Feb 2014, available
Naibaho, P.M. (1998). Teknologi Pengolahan Kelapa Sawit. Palm Oil Research Centre
Nasrin, A.B., Ma, A.N., Choo, Y.M., Mohamad, S. Rohaya, M.H., Azali A., and Zainal Z.
(2008). Oil Palm Biomass as Potential substitution Raw Materials for Commercial
Biomass Briquettes Production. American Journal of Applied Sciences 5(3): 179-
Nor Hafizah, A.B., Paridah, M.T., Yuziah, N.M.Y., Zaidon, A., Choo, A.C.Y., and
Norazowa, S. (2014). Influence of Resin Molecular Weight on Curing and Thermal
Degradation of Plywood Made From Phenolic Prepreg Palm Veneers. The Journal of
Nor Hafizah, A.B., Paridah, M.T., Hoong, Y.B., Zaidon, A., Yuziah, N.M.Y., Anwar,
U.M.K., and Shahri, M.H. (2012). Adhesion Characteristics of Phenol Formaldehyde
Pre-Preg Oil Palm Stem Veneers. Bioresources 7(4): 4545-4562.
Nordin, I. (2012). Treatability and Fluid Pathway in Oil Palm Wood and Rubberwood.
Master Thesis. University Putra Malaysia. Malaysia
Nordin, K., Jamaludin, M.A., Ahmad, M., Samsi, H.W., Salleh, A.H., and Jallaludin, Z.
(2004). Minimizing the Environmental Burden of Oil Palm Trunk Residues Through
the Development of Laminated Veneer Lumber Products. Management
Environmental Quality 15(5): 484-490.
Norralakmam, S.Y. (2007). Particleboard. In; Turning Oil Palm Residues into Products.
Research Pamphlets No 127. Forest Research Institute Industry (FRIM), Kepong,
Nyren, V. and Back, E. 1960. Characteristics of Parencymateous Cells and Tracheidal Ray
Cells in Picea Abies Karst. Svensk Papperstidning Och Svensk
Pappersfrdlingstidskrift 63(16), 501-509.
Ohmae, Y. and Nakano, T. (2009). Water Adsorption Properties of Bamboo in the
Longitudinal Direction. Wood Science Technology 43: 415-422.
Olsson, T., Megnis, M., Varna, J., Lindberg, H. (2001). Study of The Transverse Liquid
Flow Paths in Pine and Spruce using Scanning Electron Miscroscopy. The Japan
Wood Research Society. 282-288.
Paridah, M. T., Loh, Y. F., Jalaluddin, H., and Zaidon, A. (2006). Improving the
Performance of Oil Palm Trunk Plywood by Optimising the Veneer Density
Distribution. Processing on Second International Symposium on Veneer Processing
and Products. May 9 and 10, 2006. Vancouver, BC, Canada. Pp 389-396.
Parthasarathy, M.V. and Klotz, L.H. (1976). Palm wood I. Anatomical aspects. Wood
Science and Technology 10: 231-246. Springer-Verlag. New York.
Polge, H. (1966). Two Examples of the Use of Curves for Wood-Density Variation in
Studies of Tree Physiology. Memorial Society of Botany 1968: 123-128.
Poltze, M. and Niemz, P. (2011). Porosity and Pore Size Distribution of Different Wood
Types as Determined by Mercury Intrusion Porosimetry. European Journal of Wood
Products 69: 649-657.
Rahayu, I.S. (2001) Basic Properties of Vascular Bundles and Parenchyma Tissues of Oil
Palm Trunk. Unpublished Master Dissertation, Bogor Agriculture University,
Rahim, S., Abdul Razak, M.A., Zakaria, M.A. (1988). Chemical Components in Oil Plam
Trunk Influencing Wood-Cement Board Making. The 2nd
Pacific Regional Wood
Anatomy Conference Forest Products Research and Development Institute Los
Banos (College), Lahuna, Philippines, p449-455.
Rahim, S., and Khozirah, S. (1991). Utilisation of Oil Palm Trunks for Cement-Bonded
Particleboard Manufacture. National Seminar on Oil Palm Trunk and Other
Palmwood Utilization, Ming Court Hotel, Kuala Lumpur, Malaysia.
Ralph, M.N., and Magdalena, S. (2007). The Effect of Wood Extractive Content and Glue
Adhesion and Surface Wettability of Wood. Wood and Fibre Science 34(1): 57-71.
Rasiah, R. and Shahrin, A. (2004). Development of Palm Oil and Related Products in
Malaysia and Indonesia. Unpublished report. Universiti Malaya, Malaysia.
Ratnasingam, J., Nyugen, V., and Ioras, F. (2008). Evaluation of Some Finishing Properties
of Oil Palm Particleboard for Furniture Application. Journal of Applied Sciences
Richardson, B. (2002). Defects and Deterioration in Building. 2nd
Edition. Published in
Canada and USA. p81.
Satish, K. and Dobriyal, P.B. (1992). Treatability and Flow Path Studies in Bamboo Part 1.
Dendrocalamus strictusnees. Wood and Fibre Science 24(2):113-117.
Scheller, H.V. and Ulvskov, P. (2010). Hemicellulose. Annual Review of Plant Biology 61:
Schniewind, A.P. (1989). Concise Encyclopedia of Wood and Wood-Based Materials.
Pergamon Press. p248.
Sharma, S.N. (1988). Seasoning Behaviour and Related Properties of Some Indian Species
of Bamboo. Indian Forester 114(10): 613-621.
Shebani, A.N., Reene, A.J., and Meincken, M. (2008). The Effect of Wood Extractives on
The Thermal Stability of Different Wood Species. Thermochimica Acta 47(1-2): 43-
Sheshmani, S., Ashori, A., and Farhani, F. (2011). Effects of Extractives on the Performance
Properties of Wood Flour-Polypropylene Composites. Applied Polymer Science.
Shirley, M B. (2002) Cellular Structure of Stem and Fronds of 14 and 25 Years Old Elaeis
Guineensis Jacq. Master Dissertation, Universiti Putra Malaysia, Malaysia.
Shuit, S.H., Tan, K.T., Lee, K.T., and Kamaruddin, A.H. (2009). Oil Palm Biomass as a
Sustainable Energy Source: A Malaysian Case Study. Energy 34(9):1225-1235.
Siau, J.F. (1984). Transport Processes in Wood, Springer-Verlag, Berlin.
Siau, J.F. (1971). Flow in Wood, Syracuse University Press, and New York Standard book
No: 8156-50280, Catalog Card No: 70-155829; p131.
Silva, M.R.D., Machado, G.D.O., Deiner, J., and Junior, C.C. (2010). Permeability
Measurements of Brazilian Eucalyptus. Material Research 13(3): 281-286.
Siti Noorbaini, S. (2009). Effect of Cold Setting Adhesives and Glue Spread on Properties of
Oil Palm Trunk Laminated Veneers. Master dissertation. Universiti Sains Malaysia.
Sitti Fatimah, M.R., Othman, S., Hashim, R., Arai, T., Kosugi, A., Abe, H., Murata, Y.,
Mori, Y. (2012). Characterization of Parenchyma and Vascular Bundle of Oil Palm
Trunk as Function of Storage Time. Lignocellulose 1(1): 33-44.
Sjostrom, E. (1993). Wood Chemistry, Fundamentals and Applications. 2nd
Sjostrom, E. (1981). Wood Chemistry, Fundamentals and Applications. London:
Smith, D. N., and Williams, A.I. (1969). Wood Preservation by Boron Diffusion Process-
Effect of Moisture Content on Diffusion Time. Journal Institute of Wood Science 22:
Song, H. (2012). Impact of Drying Conditions, Wood Extractives and Surface to Uneven
Distribution of Preservatives in Scots Pine. Lulea University of Technology.
Stamm, A.J. (1946). Wood and cellulose science. New York: Ronal Press.
Stamm, A.J., and Loughborough, W.K. (1942). Variation in Shrinking and Swelling of
Wood. America Society Mechanical Engineering 64: 379-386.
Sulaiman, O., Hashim, R., Razak, W., Hashim, W.S., and Azmy, M. (2008). Evaluation on
Some Finishing Properties of Oil Palm Plywood. Holz Roh Werkst. 66: 5-10.
Sulaiman, O., Mohd Fahmi, A.W., Hashim, R., and Mondal, M.I.H. (2012). The Effect of
Relative Humidity on the Physical and Mechanical Properties of Oil Palm Trunk and
Rubberwood. Cellulose Chemistry and Technology 46(5-6): 401-407.
TAPPI (1999). Standards T 207 Water Solubility of Pulp and Wood. TAPPI T 207
cm 99. p1-3.
TAPPI (2007). Standards T 280 Acetone Extractive of Pulp and Wood. TAPPI T
204 cm 99. p1-3
Taylor, A.M, Gartner, B.L., and Morrell, J.J. (2002). Heartwood Formation and Natural
Durability- a review. Wood Fiber Science 34: 587-611.
Teoh, C.H. (2002) The Palm Oil Industry in Malaysia: From Seed to Frying Pan. WWF
Switzerland: WWF Malaysia.
Teutonico, J.M. (1988). A Laboratory Manual for Architectural Conservators. International
Centre for the Styudy of the Preservation and the Restoration of Cultural Property
Thuvander, F., Wallstrom, L., Berglund, L.A., Lindberg, K.A.H. (2001). Effects of an
Impregnation Procedure for Prevention of Wood Cell Wall Damage Due to Drying.
Wood Science and Technology 34: 473-480.
Tomimura, Y. (1992). Chemical Characteristics of Oil Palm Trunk. Bulletin Forestry and
Forestry Product Residue Institute 362: 133-144.
Tomlinson, P.B. (1961). Anatomy of the Monocotyledons II, Palmae. Clarendon Press
Oxford. p9 24.
Tomlinson, P.B. (1990). The Structural Biology of Palms. Oxford University Press. New
Tsoumis, G.T. (1991). Science and Technology of Wood: Structure, Properties, Utilization.
494. New York: Van Nostrand Reinhold.
Ulvcrona, T., Lindberg, H., and Bergsten, U. (2006). Impregnation of Norway spruce
(Picea abies L. Karst.) Wood by Hydrophobic Oil and Dispersion Patterns in Different
Tissues. Forestry 79(1): 1223-134.
Usta, I. (2003). Comparative Study of Wood Density by Specific Amount of Void Volume
(Porosity). Turkey Journal Agricultural Forestry 27: 1-6.
Usta, I. (2006). Comparative Characterization of the Effects of the Climate-Tree-Growth
Relationship in Anatolian Black Pine (Pinus nigra Arnold subsp. pallasiana (Lamb.)
Holmboe) on Wood Treatability. Turkey Journal of Agriculture Forestry 30: 305-
Vaickelionis, G. and Vaickelioniene, R. (2006). Cement Hydration in the Presence of Wood
Extractives and Pozzolan Mineral Additives. Ceramics-Silikaty 50(2): 115-122.
Vick, C.B. (1999). Chapter 9. Adhesive Bonding of Wood Materials. Wood Handbook.
Wood as an Engineering Material. Madison, WI, U.S. 463. W.Junk Publisher
Walinder, M. (2000). Wetting Phenomena on Wood; Factors Influencing Measurements of
Wood Wettability. Doctoral Thesis, KTH- Royal Institute of Technology,
Walker, J.C.F., and Butterfield, B.G. (1996). The importance of Microfibril Angle to the
Processing Industries. New Zealand Forestry 40: 34-40.
Wan rosli, W.D., Zainuddin, Z., Law, K.N., and Asro, R. (2007). Pulp from Oil Palm
Fronds by Chemical Processes. Industrial Crops and Products 25(1): 89-94.
Wengert, E.M. (2006). Principles and Practices of Drying Lumber. Brooks Forest Products
Center. Virginia Polytechnic Institute and State University, Virginia, USA.
Wenzl, H. (1970). The Chemical Technology of Wood. Academy Press. New York.
Whitmore, T.C. (1973). The Palms of Malaya. Longmans, Selangor, Malaysia.
Wilson, K., and D.J.B. White (1986). The Anatomy of Wood: Its Diversity and
Variability. Stobart and Son Ltd, London.
Xie, H., King, A., Kilpelainen, I., Granstrom, M., and Argyropoulos, D.S. (2007).
Thorough Chemical Modification of Wood-Based Lignocellulosic Materials in Ionic
Liquids. Biomacromolecules 8: 3740-3748.
Yamamoto, S., Nakano, T, Norimoto, M and Miyazaki J. (2005). Analysis of Water
Adsorption of Bamboos on the Basis of Hailwood and Horrobin Theory. Mokuzai
Gakkaishi 51: 372-379.
Yusof, B. (2007). Palm Oil Production through Sustainable Plantations. European Journal
of Lipid Science and Technology 109: 289-295.
Zaidon, A. (1995). The Structure and Properties of Rattan in Relation to Treatment with
Boron Preservatives. PhD. Thesis. University of Aberdeen. p222.
Zaidon, A., and Petty, J.A. (1997). Absorption of Water by Rattan (Calamus Spp.)
During Three Treatment Process. Journal of Tropical Forest Products 3(2):
Zaihan, J., Hill, C.A.S., Hashim, W.S., Mohd Dahlan, J., and Sun, D.Y. (2011). Analysis
of the Water Vapour Sorption Isotherms of Oil Palm Trunk and
Rubberwood. Journal of Tropical Forest Science 23(1): 97-105.
Zakiah, A., and Azmi, I. (2010). Drying Shrinkage Characteristics of Concrete Reinforced
with Oil Palm Trunk Fiber. International Journal of Engineering Science and
Technology 2(5): 1441-1450.
Zimmer, K., Larnoy, E., and Koch, G. (2009). Wood Properties Influencing the Penetration
of Scots Pine (Pinus sylvestris) Sapwood with the Wood Modification Agent
Furfuryl Alcohol. The International Research Group on Wood Protection Document
No IRG/WP 09-40470.
Zugenmaier, P. (2006). Materials of Cellulose Derivatives and Fiber-Reinforced Cellulose-
Polypropylene Composites: Characterization and application. Pure Applied
Chemistry 78(10): 1843-1855.
INFLUENCE OF EXTRACTIVES ON THE POROSITY OF OIL PALM(Elais guineensis Jacq.) STEMABSTRACTTABLE OF CONTENTSCHAPTERSREFERENCES